Kategory: Hot Work Tool Steel
Among the alloy tool steels, the so called hot work die steel (JIS name is SKD61) is being used as the material for the cavity or the core. It is also considered precious as a material for thin core pins because it has a relatively high hardness, withstands wear, and also has relatively high resistance to shock.
In order to bring out its excellent characteristics, SKD61 needs quenching, and after quenching, it is tempered to stabilize the metallographic texture and to improve its toughness. However, since it is known that depending on the conditions of tempering SKD61 causes change of dimensions and reduction of hardness, unforeseen failures can result if the tempering is done without understanding this trend. Therefore, in this course, the tempering characteristics of SKD61 are explained below.
Reduction in the hardness due to tempering
The hardness of SKD61 decreases in various cases by tempering after it is quenched. For example, if a material quenched at 1030°C is tempered, the following changes occur depending on the tempering temperature. (The following data is an actual example, and there will be changes depending on the size of the work and the plate thickness.)
Therefore, since the hardness decreases suddenly if the tempering is done at an unnecessarily high temperature, care should be taken when resistance to wear is necessary.
Changes in the dimensions due to tempering
The external dimensions of the work change, when SKD61 is tempered after it is quenched. Depending on the tempering temperature, the external dimensions can become larger or smaller. If additional machining is not to be done after tempering, it is necessary to carry out the machining work before quenching taking into considerations the change in the dimensions after tempering.
Example: Quenching at 1030°C
Extrusion mandrel, press and forging dies, moulds for pressure casting low density metals, ejector pins, Universal hot work tool steel,etc
Filed under: Tool Steel | Ditandai: 20 mm, 2011, 2012, 2013, 2014, 2015, 2016, 2017, 2018, 2019, 2020, 2344, 25, agen, agent, AISI, AISI Equivalents for JIS SKD61, AISI H13, aplikasi, application, Assab, ASTM Equivalents for JIS SKD61, Availability, baja, baja SKD61, berat, besi SKD61 bekas, besi SKD61 full, beyond-steel, Bohler, BOHLER W302 SUPERIOR®, Carbide, Carbon steel, catalog, Characteristic, Characteristics, chemical, Chemical Composition, chemical composition BESI SKD61, china, composition, daftar, data sheet, dia, diameter, diameter BESI SKD61, dimensi, DIN, DIN X40CrMoV51, distributor, distributor BESI SKD61, equivalent, equivalent assab, equivalent bohler, equivalent of SKD61 beam, europe, ex, feet, flat, ft, galvanis, grade Baja SKD61, h13, hardness, harga, harga BESI SKD61, harga besi SKD61 2011, harga murah, harga s45 plat, harga SKD61 roundbar baru, harga terbaru SKD61, hari ini, heat, heat treatment, hitachi, hot dip, Hot Rolled, Hot-dip galvanizing, HSS, ID BESI SKD61, impor, import, import jual, importir, Inch, indonesia, jakarta, jenis, jis, JIS SKD 61, JIS SKD61, jual, jual beli, Jual besi jual SKD61 roundbar, Jual BESI SKD61, jual besi SKD61 eks gudang, jual Besi SKD61 JIS3192, jual plat SKD61, Jual SKD61, jual SKD61 pangeran jayakarta, jual SKD61 second, ketebalan, krakatau, length, lokal, mechanical, Melting, Melting Point, meter, mild steel, mm, Nippon, of, pabrik, Physical, Plate, Point, properties, Round Bar, SAE Equivalents for JIS SKD61, size, skd 61, skd61, SKD61 Hardness, skd61 harga miring, SKD61 Mechanical Properties, SKT4, sole, spec, spesifikasi, standard, steel, stockis agen dan distributor tool steel harga murah, stockist dan importir Tool Steel SKD 11, terbaru, thickness, Thyssen 1191, thyssen 2344, Thyssenkrupp, titanium alloy, tool, Tool steel, tool steel skd61, Treatment, Tungsteen, ukuran, W302 SUPERIOR®, width, X40CrMoV51 | Leave a comment »